## Mathematical Modelling of Corrosion for Polymers

### Norazaliza Mohd Jamil

Faculty of Industrial Sciences & Technology, Universiti Malaysia Pahang, Lebuhraya Tun Razak, 26300, Gambang, Kuantan, Pahang, Malaysia

Copyright c2019 by authors, all rights reserved. Authors agree that this article remains permanently open access under the terms of the Creative Commons Attribution License 4.0 International License

### Abstract

The material of pipelines transporting water is usually polymers. Chlorine as oxidant agent is added into the water system to prevent the spread of some disease. However, exposure to a chlorinated environment could lead to polymer pipe degradation and crack formation which ultimately reaches a complete failure for the pipes. To save labor, time and oper-ating cost for predicting a failure time for a polymer pipe, we focus on its modeling and simulation. A current kinetic model for the corrosion process of polymers due to the action of chlorine is extensively analyzed from the mathematical point of view. By using the nondimensionalization method, the number of parameters in the original governing equations of the kinetic model has been reduced. Then, the dimensionless set of differential equations is numerically solved by the Runge Kutta method. There are two sets of simulations which are low chlorine concentration and high chlorine concentration, and we captured some essential characteristics for both types. This approach enables us to obtain better predictive capabilities, hence increasing our understanding of the corrosion process.### Keywords

Corrosion, Kinetic Model, MathematicalModelling, Dimensionless

### 1

### Introduction

Corrosion on polymers can be obviously seen when there is crack on the polymer surface. However, the corrosion on the polymer is often hard to discover where the material looked normal but internally the strength of the material is weak. In physical testing, it is hard to determine the state of the material and to decide when the maintenance need to take place. To make things worse, sometimes after an accident occurred, then we realized that there is corrosion. To save labor and time, and for the safety purpose, simulation of the corrosion process is necessary to test various conditions and determine the failure time of the pipe. Colin [1] presented a satisfactory prediction of molecular weight loss during the corrosion process. Here in this paper, his kinetic model is extensively studied to analyze the oxidant and antioxidant concentration profiles in polymer pipes.

Deterioration of polymer is one of the main concerns for people working with pipelines industry. A significant effort has been devoted to studying the corrosion due to environmen-tal conditions. Compared with pipes made from other material, the polymer is an anti-corrosion material and low cost com-pared to metal. Even the polymer is an anti-corrosion material, the exposure to oxidant agent, high pressure and temperature affect the performance of the polymer. The process of poly-mer corrosion consists of chemical reaction, diffusion, and me-chanical deformation. The chronology of corrosion of polymer pipes due to chemical aging is as follows [3]: (a) A polymer is exposed to chlorine (oxidant agent/disinfectants). (b) The an-tioxidant is added to prevent corrosion. (c) Anan-tioxidant react to the oxidant agent. (d) Antioxidant disappeared slowly (migra-tion). (e) Oxidant absorbs on the polymer surface. (f) Polymer reacts to oxidant directly causing to chain scission and make the molecular chain shorter. Hence, the cause of polymer cor-rosion is radical chain-oxidation [5].

Polymer pipes that transporting water will undergo failure after a certain time due to the physical and chemical aging. The water contains two reactive species which are oxygen and disinfectants (chlorine dioxide). Disinfectants will destroy or-ganic compounds, often by radical processes. It degraded the inner surface of plastics pipelines, developed cracked and even-tually reach a complete failure. The lifetime of a pipeline is normally 50-100 years, however, these factors make the degra-dation goes faster so that the lifetime becomes shorter i.e. 1-25 years [3].

The complexity of corrosion processes creates the neces-sity for a quantitative model approach to developing predictive tools, which simultaneously provide both quantitative informa-tion as well as simulainforma-tions of the various processes involved.

The kinetic equations of polymer corrosion have been ex-tensively studied and many kinetic models have been proposed [1][2]. The mechanisms of polymer degradation induced by chlorine dioxide in terms of the kinetic model have been estab-lished by [1]. Ge et al. [3] developed a model to investigate the time-dependent crack propagation in a viscoplastic poly-mer. Their result shows that failure behavior is dependent on the applied load.

The objective of this research is to analyze the oxidant and antioxidant concentration profile in polymer pipes. By analyz-ing these components, the primary aganalyz-ing process of the pipes

can be understood. We analyzed the problem using a mathe-matical model developed by in [1].

This paper deals with the effect of chlorine dioxide (DOC) on the aging of polyethylene (PE) pipes for the transport of wa-ter. DOC which is a free radical can initiate radical chain ox-idation in PE. Oxox-idation in-duces random chain scission, and this latter leads to embrittlement when the weight average mo-lar massMw becomes typically lower than 70 kg mol−1. A

mechanistic scheme for low-temperature PE thermo-oxidation incorporating DOC reactions has been built [1].

In this paper, a nondimensionalization is presented for the governing equations of polymer corrosion kinetic model de-scribed in [1]. Using a nondimensionalization of these equa-tions, a number of nondimensional group parameters are pro-posed. Structurally, this paper consists of for thematic sections with relevant subsections. In the first section, we introduce the paper. The second section is concerned solely on the mechan-ics of the nondimensionalization, where we introduce a mathe-matical analysis for the model. In the third section, we discuss the solutions. Finally, the conclusion of this paper is provided.

### 2

### Mechanics of the

### Nondimensionaliza-tion

The oxidation processes occurring on polymer pipes when exposed to chlorine dioxide. In this section, we aim to in-troduce a mathematical model able to describe the corrosion effects on a polymer layer, which is subject to deposition of chlorine. The present model is based on the mathematical ap-proach used in [1]. The ten governing equations of the kinetic model for corrosion for polymers were presented in [1].

The complexity of the system makes finding the analytical solution difficult. To solve the system of equations, we per-haps have to resort to numerical methods that can incur sig-nificant computational cost. Our strategy here is to look for reduced order models by ignoring significantly small terms in the governing system of equations. The goal is to ensure that mathematical results are consistent with physical requirements. Reformulating a model in dimensionless form is beneficial from several aspects. This procedure can help to check the consistency of the model equations and confirm that all terms have the same set of units in a differential equation. In addi-tion, nondimensionalizing a model reduces the number of free parameters and reveals a smaller set of quantities that govern the dynamics. Once a model is dimensionless, it shows which terms have a larger or smaller magnitude, which can help to obtain approximate solutions using techniques such as asymp-totic analysis. Table 1 represents the unit of each variable.

There are eleven fundamental scales; all others can be de-rived from these scales. These nondimensional parameters and the scales that they are based upon are:

τ = t t0

,[doc] = [DOC] Cin

,[ah] = [AH] Hin

,[o2] = [O2] Gin

,

[ph] = [P H] P Hin

,[pooh] = [P OOH] P OOHin

,[po2] = [P O

•

2]

[image:2.595.304.538.100.499.2]P OOHin

Table 1.Parameter units

Parameters Units

DOC, AH,O2, PH, POOH,P O2•,P O•2 moll−1

Q, s, x moll−1

k1b, k1d, k1s, ks1, k2, k3, k4, k5, k6a, k7 lmol−1s−1

k1u, k6b, k6c, k6d s−1

nAH, γ1s, γ4, γ5 no unit

[p] = [P

•_{]}

P OOHin

,[q] = [Q] P OOHin

,s˜= s s0

,x˜= x x0

where tis time,

t0is the characteristic time,

DOCis chlorine dioxide solution,

Cinis initial value of chlorine dioxide solution,

AHis stabilizer,

Hinis initial value of stabilizer,

O2is oxygen,

Ginis initial value of oxygen,

P His polyethylene,

P Hinis initial value of polyethylene,

P OOHis hydroperoxides,

P OOHinis initial value of hydroperoxides,

P O•_{2}is radical,
P•is radical,

Qis caged pair ofP O•_{2}radical,

nAHis phenolic stabilizer functionality,

sis quantity of chain scission, xis quantity of crosslinking, and

Therefore, we obtained a dimensionless system as follows. d[doc]

dτ =−k1dP Hin[doc][ph]−nAHk1sHin[doc][ah] −k7P OOHin[doc][p]

d[ah]

dτ =−nAHk1sCin[doc][ah] −nAHks1P OOHin[po2][ah]

d[o2]

dτ =−k2P OOHin[O2][p] +k6aP OOHin/Gin[po2]

2

d[ph]

dτ =−(2 +γ1s)P OOHin/P Hink1u[pooh] −(1 +γ1s)k1bP OOHin2/P Hin[pooh]2

−k1dCin[doc][ph]−k3P OOHin[ph][po2]

+2γ4k4P OOHin2 /P Hin[p]2

+(3γ5−1)k5P OOHin2/P Hin[p][po2]

+2k6bP OOHin/P Hin[q]

−2(1 +γ1s)k6dP OOHin/P Hin[q]

d[pooh]

dτ =−k1uy(5)−2k1bP OOHin[pooh]

2

+k3P Hin[ph][po2] + (1−γ5)P OOHin[p][po2]

d[po2]

dτ =k1bP OOHin[pooh]

2_{+}_{k}

2Gin[o2][p]

−k3P Hiny(4)[po2]−k5P OOHin[p][po2]

Table 2.Parameter values for elementary rate constants

Parameters Value

γ1s 1

γ4 0.5

γ5 0.0108

k1b 8.6×10−9

k1d 2.7×10−5

k1u 3.6×10−11

k2 108

k3 10−2

k4 8×1011

k5 1.6×1011

k6a 2.2×106

k6b 2×106

k6c 1.8×105

k6d 6×106

k7 2×106

PHin 60

POOHin 10−2

Pin 0

PO2in 0

Qin 0

d[p]

dτ = 2k1u[pooh] +k1bP OOHin[pooh]

2

+k1dCinP Hin/P OOHin[doc][ph]

−k2Gin[o2][p] +k3P Hin[ph][po2]

−2k4P OOHin[p]2−k5P OOHin[p][po2]

+2k6d[q]−k7Cin[p][doc]

d[q]

dτ =k6aP OOHin[po2]

2_{−}_{(}_{k}

6b+k6c+k6d)[q]

d[s]

dτ =γ1sk1uP OOHin[pooh] +γ1sk1bP OOH

2

in[pooh]

2

+2γ1sk6dP OOHin[q]

d[x]

dτ =γ4k4P OOH

2

in[p]2+γ5k5P OOHin2[p][po2]

+k6bP OOHin[q]

The reduction in the number of parameters makes theoret-ical manipulation easier, as the equations are less cluttered. We solved the set of dimensionless system of differentiable equations using Runge Kutta method. The parameter values is recorded in Table 2 where we refer [1].

### 3

### Results and Discussion

To gain an understanding of the kinetic model, we ob-serve the changes in the behaviour of the system. We fixed the initial concentration of stabiliser and studied how the dynamic change with varying DOC concentration. We assumed the initial concentration of stabiliser is 8.5 mol/l in all simulation study. Elementary rate constants γ1s, γ4, γ5, k1b, k1d, k1u, k2, k3, k4, k5, k6a, k6b, k6c, k6d, k7

and initial values P Hin, P OOHin, Pin as recorded in

Ta-ble 2 have been previously determined in [4] and will be used here without modification. In all simulation, we set

nAH= 1, k1s= 1, ks1= 1,sin= 1xin= 1,Hin= 8.5, and

Gin= 20.

[image:3.595.315.541.263.635.2]To get insight into the behavior of chlorine and stabilizer, we plot the graphs in Figure 1. In this graph, we set the initial con-centration of DOC is 3 mol/l (low DOC concon-centration). At low DOC concentration, according to Figure 1, the profile of chlo-rine and stabilizer decreased within a short time and then lev-eling off. The small amount of chlorine depleted and dropped to zero due to the action of the stabilizer. Chlorine dioxide initiates polymer oxidation. Hence, the numbers of chain scis-sion increased throughout the time before it reached a steady state. The presence of chlorine accelerates the consumption of stabilizers and consequently the degradation of polymer pipes.

Figure 1. Low DOC concentration (a) The profile of chlorine and stabiliser

concentration (b) The number of chain scission and crosslink when Hin=8.5 and Cin=3.

Figure 2 shows the concentration profiles of chlorine and stabilizer at high DOC concentration i.e. Cin = 10. At high

due to the action of the stabilizer but it remain in the system. Both of the numbers of chain scission and crosslinks increased concerning time before it reached the steady state. Polymer degradation started when the antioxidant system was depleted.

Figure 2. High DOC concentration (a) The profile of chlorine and stabiliser

concentration (b) The number of chain scission and crosslink when Hin=8.5 and Cin=10.

Figure 3 shows the profile of chlorine concentration for dif-ferent initial values of DOC i.e.Cin= 3,10,20. As the initial

DOC concentration is higher, the longer the DOC will remain in the system. For a low initial value of DOC, the chlorine de-pleted rapidly due to the action of stabilizer. On the other hand, Figure 4 indicates that the concentration of stabilizer varies for the various value ofCin. AsCingetting higher, the amount of

stabilizer remained in the system is lower. The loss of stabi-lizer from the system is to increase asCinincreased. The time

of depletion of antioxidant is shorter asCinincrease. The

con-sumption of antioxidants in polyethylene containing different chlorine concentrations are the subject Figure 4.

As Cin getting higher, the number of chain scission is

[image:4.595.56.279.155.534.2]higher, as illustrated in Figure 5. Similarly, the number of crosslink increase when the amount of chlorine added to the system increased (Figure 6).

Figure 3. The profile of chlorine concentration for different initial value of

DOC.

Figure 4. The profile of stabiliser concentration for different initial value of

[image:4.595.317.540.339.518.2]DOC.

[image:4.595.313.539.575.757.2]Figure 6.The number of crosslinks for different initial value of DOC.

### 4

### Conclusion

In this paper, we employed the nondimensionalization tech-nique for the kinetic model of corrosion process of polymer pipes that exposed to the chlorinated environment. We re-duced the complex model to a set of simple equations. The behavior of the model between the high-concentrated initial value of chlorine dioxide and low-concentrated one is com-pared. We studied the effect of different DOC concentration on the model. The resulting approximate solutions capture some essential characteristics and provide insights into the system. This approach enables us to predict corrosion behavior without the necessity of extensive use of laboratory testing. It is found that mathematical analysis is in agreement with the laboratory

experiments recorded in the literature.

### Acknowledgements

The author gratefully acknowledged the financial supports received from FRGS (RDU 160116)(Ref: FRGS/1/2016/STG06/UMP/02/3).

### REFERENCES

[1] Colin X, Audouin L, Verdu J, Rozental-Evesque M, Rabaud B, Martin F, Bourgine F (2009) Aging of polyethylene pipes trans-porting drinking water disinfected by chlorine dioxide. I. Chem-ical aspects. Polymer Engineering & Science, 49(7), 1429-1437.

[2] Colin X, Audouin L, Verdu J, Rozental-Evesque M, Rabaud B, Martin F, & Bourgine F (2009) Aging of polyethylene pipes transporting drinking water disinfected by chlorine dioxide. Part II—Lifetime prediction. Polymer Engineering & Science, 49(8), 1642-1652.

[3] Ge H, Le J L, & Mantell S C (2016). Numerical modeling of stress corrosion cracking of polymers. Engineering Fracture Mechanics, 160, 199-21.

[4] N. Khelidj, X. Colin, L. Audouin, J. Verdu, C. Monchy-Leroy, and V. Prunier, Polym. Deg. Stab., 91(7), 1593 (2006).2.

[5] Colin & Minard, Chemical degradation of polyethylene pipes due to water-based disinfectants.